Solidification and Solid State Phase Transformation of Allvac 718Plus Alloy
Embed Size (px)
Transcript of Solidification and Solid State Phase Transformation of Allvac 718Plus Alloy
SOLIDIFICATION AND SOLID STATE PHASE TRANSFORMATION OF ALLVAC 718PLUS ALLOY
ATI Allvac, an Allegheny Technologies Company, 2020 Ashcraft Avenue, Monroe, NC 28110, USA
Keywords: 718Plus, Solidification, Aging, G phase
Solidification and solid state transformations of Allvac 718Plus alloy were studied by modeling and experiment. Solidification behavior was investigated by DTA and SEM/EDS techniques and compared with modeling calculations. Various phases were identified and formation of the cast structure was interpreted on the basis of a pseudo-binary phase diagram developed in this work. The chemistry, crystal structure and growth rate of hardening phases and their precipitation kinetics were studied. Aging behavior and the effect of solution temperature and plastic deformation were addressed. Special attention was paid to G phase precipitation. The nature, morphology and formation kinetics of G phase were investigated and its effect on mechanical properties are discussed.
In recent decades, an effort has been made to develop a Ni-base superalloy that has temperature capability at least 55C higher than that of alloy 718 with 718-like processability and a cost lower than that of alloys applied at equivalent temperatures such as Waspaloy. As part of this effort, a new alloy, Allvac 718Plus, was developed at ATI Allvac . The chemistry of this alloy was determined by detailed modeling and experimental studies and the results have been reported . Much experimental work demonstrated that this alloy has excellent mechanical properties up to 704C, processability approaching that of alloy 718 and cost lower than alloys such as Waspaloy and Ren 41 [3-4]. The chemistry of this alloy, together with alloys 718 and Waspaloy is shown in Table I.
Table I. Nominal Chemistry Comparison of Alloys 718Plus, 718 and WaspaloyChemistry, wt% Alloy
C Cr Mo W Co Fe Nb Ti Al P B718Plus 0.025 18.0 2.70 1.0 9.0 10.0 5.40 0.70 1.45 0.007 0.004
718 0.025 18.1 2.90 18.0 5.40 1.00 0.45 0.007 0.004Waspaloy 0.035 19.4 4.25 13.25 3.00 1.30 0.006 0.006
Like other superalloys, the processing of alloy 718Plus, especially solidification, hot working and heat treatment practices, has to be carefully controlled to generate a desirable microstructure and therefore the required mechanical properties. A thorough understanding on the relationships among processing, microstructure and mechanical properties is very critical to the application of this alloy. This type of study obviously requires many years effort by many researchers, as shown in some highly successful alloys such as 718. Therefore, only a few relevant topics could
Superalloys 718, 625, 706 and Derivatives 2005 Edited by E.A. LoriaTMS (The Minerals, Metals & Materials Society), 2005
be addressed in this study and the results must be preliminary in nature. Solidification structure,J'/J" precipitate state and G phase precipitation among others play a very critical role in formingthe mechanical properties of this alloy. This paper will concentrate on these issues and briefly introduce the results of relevant studies.
Solidification structure, including macro-, microsegregation and various eutectic reactions,significantly influence the mechanical properties of wrought products, and the behavior in solidification will determine the size of ingot that can be readily made from this alloy. The behavior during solidification was investigated by modeling calculations, differential thermalanalysis (DTA) and detailed SEM/EDS study of the cast structure.
Modeling analysis of the solidification process was conducted, using the JMatPro software tool, on both alloys 718 and 718Plus. A comparison was made of the solidification temperature range, Nb segregation and carbide formation of both alloys. As shown in Table II, both alloys have similar liquidus, solidus and, therefore, solidification temperature ranges with those of alloy 718Plus being slightly lower. Segregation of Nb in alloy 718Plus is actually slightly lower than alloy 718 although both have the same Nb content. The carbide precipitation in both alloys are also very similar.
Table II. Modeling Results of Solidification Characteristics of Alloys 718Plus and 718 Solidification Temperature
CNb Segregation MC Carbide Precipitation
TSTL - TS
Nb in liquid at Solidus
MC at Solidus
718Plus 1346 1201 145 0.40 13.43 % 1260 0.160 % 718 1358 1214 144 0.35 15.42 % 1267 0.155 %
The freckle tendency of various Ni-base superalloys has been calculated using Rayleigh numbercriterion . As Figure 1 shows, alloy 718Plus has similar freckle tendency to alloy 718 and 625.
1000 1200 1400 1600 1800 2000
718 718+ 625 706 Waspaloy
Figure 1. Rayleigh Criterion Segregation Tendency for Various Wrought Ni-Base Alloys.
Waspaloy has the highest freckle tendency among all alloys calculated. This, coupled with the data in Table II, suggests that the capability of alloy 718Plus for making large size ingot mightbe similar to that of alloy 718 and better than Waspaloy.
Differential Thermal Analysis (DTA) Study
To clarify non-equilibrium behavior, a DTA study was conducted on alloy 718Plus. A comparison with data on alloy 718  is made in Table III. It shows that both alloys have quitesimilar behavior in a non-equilibrium condition. Both alloys showed a Laves eutectic reaction at similar temperatures during solidification. This eutectic could be eliminated by long timehomogenization because Laves eutectic reaction did not show up in the DTA on-heating cycle of homogenized material and was only seen in the on-cooling solidification cycle. It appears that DTA gives a higher liquidus for alloy 718Plus and higher solidus for both alloys, which meansthe solidification range drops from 145C (modeling) to 88C (DTA) for alloy 718Plus and from144C (modeling) to 110C (DTA) for alloy 718.
Table III. Critical Phase Transformation Temperatures of Alloys 718Plus and 718 Modeling DTA MetallographyPhase
Liquidus 1346 1358 1353 1345 MC Eutectic 1261 1246 1292 1286
Solidus 1201 1214 1265 1235 1230Laves Eutectic 1173 1167 1165G Solvus 1065 1027 1002- 1018 996- 1015J' Solvus 995 909 963 936 954- 982 J" Solvus 968 946
As-Cast Microstructure and Pseudo-Binary Phase Diagram
As-cast microstructure of a 500-mm VIM/VAR ingot is shown in Figure 2. It consists of a dendrite structure with Nb-Ti carbide or carbo-nitride eutectics and two types of Laves eutectics, very similar to that of alloy 718. A detailed SEM/EDS study was conducted to identify the phases in cast structure and the results are listed in Table IV. Metallographicanalysis showed that there are less Laves eutectics in alloy 718Plus than in alloy 718.
(a) (b) (c)
Figure 2. As-Cast Microstructure of Alloy 718Plus (a) As-Cast Structure, (b) Laves Eutectics I and (c) Laves Eutectics II.
Table IV. Chemistry of Laves and MC Carbides in Alloys 718 and 718Plus Chemistry (Metal elements only), wt% Phase Alloy Method
Ni Co Cr Fe Mo W Nb Al Ti718 EDS 39.5 13.5 13.2 5.8 26.5 0.3 0.9
EDS 35.2 9.4 11.8 6.2 5.6 1.1 29.7 0.3 0.6
Modeling 0 0.02 0.2 95.9 0 2.9EDS Nb-enriched)
3.3 1.7 1.2 3.4 86.3 0 7.4718EDS (Ti-enriched)
1.4 0.7 0.8 0.7 32.6 0 63.1
Modeling 0 0 0.06 0 0.3 0.1 96.1 0 3.2EDS Nb-enriched)
2.6 0.5 0.8 0.6 0.8 0.5 81.1 0 13.1
3.6 0.6 1.7 0.7 0.1 0.2 23.3 0 69.7
In order to understand the formation of cast structure better, extensive EDS work was carried out to construct a pseudo-binary phase diagram illustrated in Figure 3. The solid lines in this figure illustrate the approximate equilibrium borderlines and the dotted lines at the left part of the diagram show non-equilibrium borderlines at actual solidification conditions. The formation of Laves eutectics and its elimination by homogenization can be easily understood from this figure. Compared to similar published figures [7, 8] and our own results for alloy 718, less Laves eutectics in alloy 718Plus can be explained. Less Laves phase in this alloy may also be associated with lower iron content.
0 5 10 15 20 25 30 35
Nb Content, wt%
~ 4.7%9.3% 23.6% 29.6
Liquid + J
J J + Laves'
Figure 3. Pseudo-Binary Phase Diagram of Alloy 718Plus
Hardening Precipitates and Aging Behavior
As reported in ref. , alloy 718Plus is predominantly strengthened by J phase in contrast with alloy 718 strengthened mainly by J" phase. Therefore, the precipitation hardening behavior of alloy 718Plus would be different from alloy 718. The nature of hardening phases, their precipitation kinetics, and growth and transformation of precipitates during thermal exposure
was studied by modeling and various experimental techniques. The aging process and the effect of solution temperature and plastic deformation were also investigated.
Precipitation Hardening Phases
The modeling results of precipitation har